Focused ion beam (FIB). Overview. Ion source and optics. Ion-solid interaction, damage. Scanning ion beam imaging. ECE 730: Fabrication in the nanoscale : principles, technology and applications Instructor: Bo Cui, ECE, University of Waterloo; http://ece.uwaterloo.ca/~bcui/
Ion source and optics.
Ion-solid interaction, damage.
Scanning ion beam imaging.
ECE 730: Fabrication in the nanoscale: principles, technology and applications
Instructor: Bo Cui, ECE, University of Waterloo; http://ece.uwaterloo.ca/~bcui/
Textbook: Nanofabrication: principles, capabilities and limits, by Zheng Cui
FIB is based on similar technology as SIMS
Primary ion beam
Secondary Ion Mass Spectrometry (SIMS) is a analytical tool with high spatial resolution and high sensitivity.
It uses a highly focused ion beam (generally oxygen or cesium ions for inorganic samples) which “sputters” material from a selected area on sample surface.
The ejected “secondary ions” pass through a mass spectrometer, which separates the ions according to their mass/charge ratio, in effect providing chemical analysis of a very small sampling volume.
Energy E=½mv2 momentum=mv=(2mE)1/2m1/2 for same E.
Gun with LMIS ion source
Ion current selection aperture
Mass selection aperture
Faraday cup (measure current)
Early ion sources were developed for mass spectrometry and nuclear physics research, then for ion implantation for semiconductor manufacturing.
Electron bombardment ion sources. Gas molecules bombarded by electrons become ionized, producing a stream of ions. Small ion current and small ion energy spread, used in mass spectrometry.
Gas discharge ion source. High current, used in nuclear physics instrumentation such as high energy accelerators and ion implanters.
Field ionization source. Gas molecules absorbed on the surface of a fine needle tip can be directly ionized at extremely high electrical field near the tip apex. Used as field ion microscope to study atomic structure of a material.
Liquid metal ion source (LMIS). A field emission source from liquid metal under a strong electrical field.
The W wire is not sharp at all!
LMIS emitter substrate
The W wire is not sharp at all!
But the “Taylor” cone of the liquid metal induced by electric field is very sharp.
As a result, electric field at cone apex is very high for field emission.
LMIS emitter substrate with AuGe Taylor cone
Driesel W, Dietzsch C, Muhle R, J. Vac. Sci. Technol. B, 14, 3367(1996)
Liquid metal ion source
Blunt W with grated
surface for Ga transport
Ga forms a Taylor cone
Force independent of m, same for electron and ion.
v is speed, much smaller for ions than for electrons; so much smaller force, need impractically large B to focus.
V is acceleration voltage.
Spot size 20nm at 100pA.
For electron, spot size < 10nm at 1000pA.
Three regimes of ion-solid interactions
Regime I (knock-on regime)
M1<<M2 or E0 is low, minimum sputtering
Regime II (linear cascade regime), where FIB operates.
M1M2, E0 is moderate, governed by nuclear effects
Regime III (spike-on regime)
M1>M2 and/or E0 is high, majority of atoms move in collision cascade
Ion range (penetration/ attenuation depth)
Ion range varies with ion energy and substrate material, order 1nm/keV
(for electron, a few m at 30keV)
30 keV Ga+ on W/Si sample
Penetrate deeper inside Si than W
Grazing angle, less damage, fast milling rate
T. Ishitani, et al., J. Vac. Sci. Technol. B16, 1907 (1998)
InP, 40nm damage/amorphization layer thickness
10 keV 30 keV
Si 6 nm 28 nm
GaAs 4 nm 24 nm
InP 15 nm 40 nm
J. F. Walker and R. F. Broom, Inst. Phys. Conf. Ser. 157, 473 (1996)
Reduced amorphous layer with reduced FIB energy
What material? GaAs?
30keV 5keV 2keV
21nm 2nm 0.5-1.5nm
One can start with high energy that mills faster, then reduce energy.
Scanning ion microscope (SIM)
Problem with FIB imaging resolution: if an object is small enough, it will be sputtered away before sufficient signal (secondary electrons) can be collected to resolve it.
Image resolution (nm)
After 1min imaging
Sputtering rate (m3/nC)
Orloff et al., JVST (1996)
Scanning ion microscopy (SIM)
Secondary electron (not ion) image
SEM (secondary electron (SE) image)
Relative secondary electron (not ion) intensity
“Origin of material contrast in scanning ion microscope”, J Electron Microscopy, 2002.
SE cannot escape, dark region
Bridging open contact with metal deposition indicates contacts at top half are good.
Open contact shown by charging. (top half charged, so is dark)
Typical SE intensity with respect to tilt angle for Fe single crystal sample under 30keV Ga-FIB bombardment.
Left: not aligned with crystal direction
Right: channeled (aligned, darker)
Ion channeling contrast